International Journal of Advanced Engineering Research and Science (IJAERS) https://dx.doi.org/10.22161/ijaers/3.11.30
[Vol-3, Issue-11, Nov- 2016] ISSN: 2349-6495(P) | 2456-1908(O)
Fatigue Crack Growth Life Prediction of 6061 AlAlloy under Load Ratio Effect by Using ANFIS J. R. Mohanty Department of Mechanical Engineering, Veer Surendra Sai University, Burla, Sambalpur 768018, India Abstract—Fatigue crack growth under constant amplitude loading for a particular material strongly depends on load ratio (R). The prediction of fatigue crack growth life under such situation through deterministic approach is a tedious task. Application of artificial intelligence methods is more encouraging in those complex situations. In the present work a novel soft-computing approach i.e. adaptive neurofuzzy technique (ANFIS) has been applied to predict fatigue life of 6061 (AA 6061) aluminum alloy under the influence of load ratio. It has been observed that the ANFIS model predict the fatigue life of the alloy reasonably well with percentage deviation of –0.024 and prediction ratio of 1.025. Keywords—Adaptive neuro-fuzzy inference system (ANFIS); fatigue crack growth rate (FCGR); root mean squre error (RMSE); prediction ratio. I. INTRODUCTION Fatigue failure is an important mode of failure which occurs in almost all engineering structures/components. There are several approaches such as fail-safe, safe-life and damage tolerant approaches in fatigue literature to deal with the fatigue phenomena. Out of those, the damage tolerant approach is one of the modern approaches based on fracture mechanics principle which mainly correlate fatigue crack growth with life (i.e. No. of cycle to failure) of the specimen. In this approach the crack growth rate (da/dN) is correlated with different material parameters and above all the crack driving forces to determine fatigue life of the computing is a good alternative for handling those complex problems as it is tolerant of imprecision, uncertainty and partial truth. As such, different soft-computing methods such as, artificial neural network (ANN), genetic algorithm (GA), fuzzy logic and adaptive neuro-fuzzy inference system (ANFIS) are being used in various fields including fatigue [9-12]. However, the prediction of fatigue life considering load ratio effect using ANFIS is rare in fatigue literature. Therefore, in the present work an attempt has been made to evaluate the constant amplitude fatigue life of 6061 aluminum alloy under load ratio effect by using www.ijaers.com
components. It can be represented by the functional form as: da (1) = f (∆K , K , R, E......) max
Based on this, several deterministic models [1-4] have been proposed till date to predict fatigue crack growth life to schedule inspection intervals for repairing/replacement of the components to avoid untimely catastrophic failures. However, the fatigue life prediction from those models suffers from several drawbacks. One of the major drawbacks is that the calculation of fatigue life from any prediction model involves complicated numerical integration schemes. Further, to formulate a fatigue model, several coupon tests are required which are not only costly but time consuming. In order to avoid those shortcomings, recently the researchers are taking the help of different computational techniques to predict fatigue crack growth life. Fatigue crack growth under constant amplitude loading for a particular material strongly depends on load ratio (R) which is the ratio of minimum load (Pmin) to maximum load (Pmax). It has tremendous effect on fatigue crack growth. Some fatigue experts [5-8] have investigated its effect on fatigue crack growth and also proposed different empirical and semi-empirical models to evaluate fatigue life. However, problems associated with fatigue are difficult to solve using conventional mathematical models because of non-linearity, noise, cost, time constraint and above all the associated micro-mechanisms. Hence, softANFIS technique. It has been observed that the proposed soft-computing technique predicts the fatigue life reasonable well with percentage deviation of –0.024 and prediction ratio of 1.025. II.
EXPERIMENTATION AND DATA PREPARATION Fatigue crack growth experiment The material under investigation was 6061 aluminum alloy received in T6 heat treated condition from rolled palte of 15 mm thickness. It was supplied by HINDALCO Industries Page | 199
International Journal of Advanced Engineering Research and Science (IJAERS) https://dx.doi.org/10.22161/ijaers/3.11.30 30 Ltd., Hirakud, Distt. Sambalpur (Odisha), India. The chemical composition of the alloy as certified by the supplier is given in Tables 1. Table.1: Chemical Composition of 6061 T6 Al Al-alloy ElemCu M Mn Fe Si Cr Al ents g Wt. % 0.15 0.8– 0.14 <0.0 0.30.3 0.04 Ba – 0.4 1.1 max 2 l 0.7 0.35 The compact tension (CT) specimens for fatigue crack growth rate (FCGR) determination were machined in the longitudinal direction with notch perpendicular to rolling direction as per ASTM E-647-99 99 standard  as shown in Fig. 1. Both the sides of the specimen were mirror polished in order to facilitate the observation of crack growth. The FCGR (da/dN)) tests were conducted on as-received as condition of AA 6061 T6 alloy as per ASTM E647 standard on a servo-hydraulic test machine (Instron Instron-8502) having a load capacity of 250 kN in air at room temperature. Initially, the specimens were fatigue pre-cracked pre under mode-II loading with a sinusoidal waveform up to a crack length to width (a/w) ratio of 0.3 under given loading conditions (frequency: 6Hz; load ratio: 0.1). Then the specimens were subjected to FCGR tests ests under constant amplitude technique (i.e. ΔK increasing) maintaining different load ratios (R)) of 0, 0.2, 0.4, 0.5, 0.6, 0.8 respectively separately and the test data were recorded. The crack growth was monitored with the help of a COD gauge mounted on the face of the machined notch.
a j = ai e
mij ( N j − N i )
aj ln ai mij = (N j − N i )
[Vol-3, Issue-11, Nov- 2016] ISSN: 2349-6495(P) 2349 | 2456-1908(O) (2)
where, ai and aj = crack length in ith step and jth step in ‘mm’ respectively, Ni and Nj = No. of cycles in ith step and jth step respectively, mij= specific growth rate in the interval i-j, i = No. of experimental steps, and j = i+1 The values of specific growth rate ‘m ‘ ij’ were calculated according to the equation (3) (3 and subsequently refined by curve fitting with calculated a values (i.e. crack lengths from initial to final with an increment of 0.005mm). 0.005mm) The smoothened values of the number of cycles were calculated in the excel sheet from the refined ‘m ‘ ij’ values as per the following equation. aj ln a N j = i + Ni mij
Then the he crack growth rates (da/dN) (d were determined directly from the above calculated values of ‘N’ ‘ as follows: ( ) a − a da (5) i = j dN
− Ni )
The superimposed crack length (a) ( vs. number of cycle (N) and nd the corresponding log (da/dN) (d vs. log (∆K) curves at different load ratios were plotted in Figs. 2 and 3 respectively.
N curves for different load ratios Fig. 2: Comparison of a–N
Fig. 1: Compact tension (CT) specimen geometry Crack growth rate determination After the fatigue crack growth rate tests, raw a – N laboratory data were obtained under each load ratio which usually contained much scatter. In order to smoothen the test data and to determine the fatigue crack growth rate, the following procedures were adopted by applying the concept of authors’ previously proposed exponential . The experimental a – N data were fitted with the th following exponential equation as per the previous model. www.ijaers.com
Fig. 3: Comparison of log (da/dN) (d – log (ΔK) for different load ratios Page | 200
International Journal of Advanced Engineering Research and Science (IJAERS) https://dx.doi.org/10.22161/ijaers/3.11.30 III. ANFIS: METHODOLOGY The fuzzy inference system (FIS) is generally used as a suitable tool for approximating ill-defined nonlinear functions. It can implement qualitative aspects of human knowledge and reasoning by using following four functional components as shown in Fig. 4. • A rule base containing a number of fuzzy if-then rules. • A decision-making unit as the inference engine. • A fuzzification interface which transforms crisp inputs to linguistic variables. • A defuzzification interface converting fuzzy outputs to crisp outputs. Adaptive neuro-fuzzy inference system (ANFIS) is an integrated system of artificial neural network (ANN) and fuzzy inference system (FIS) and utilizes the advantages of both. ANFIS is a class of adaptive networks, whose membership function parameters are tuned (adjusted) using either a back-propagation algorithm or hybrid algorithm based on a combination of back-propagation and least
[Vol-3, Issue-11, Nov- 2016] ISSN: 2349-6495(P) | 2456-1908(O)
squares estimate (LSE). In the present investigation, type-3 ANFIS  topology based on first-order Takagi-Sugeno (TSK)  if-then rules has been used.
Fig. 4: Fuzzy Inference System The structure of proposed ANFIS model consists of a number of interconnected fixed and adjustable nodes corresponding to first-order TSK fuzzy model as shown in Fig. 5. It is composed of five layers having three inputs and one output. Bell-shaped membership function has been chosen for the present investigation because it is the best membership function type . A hybrid-learning algorithm is applied to adapt the premise and consequent parameters to optimize the network. Heuristic rules are used to guarantee fast convergence.
Fig. 5: Structure of the ANFIS model IV. APPLICATION DESIGN It is known that fatigue crack growth life decreases as load ratio increases . Accordingly, the maximum stress intensity factor (Kmax), and the stress intensity factor range (ΔK) are also affected by load ratio. Therefore, during model formulation load ratio (R), maximum stress intensity factor (Kmax), and stress intensity factor range (ΔK) were www.ijaers.com
selected as linguistic input variables whereas, crack growth rate (da/dN) was taken as output variable. A set of linguistic rules formulated in the “If-Then” form were derived from expert observation and experimentation. The experimental data base consisted of six sets of fatigue crack growth data having load ratios (R) of 0, 0.2, 0.4, 0.5, 0.6 and 0.8. Each set for a particular load ratio contained Page | 201
International Journal of Advanced Engineering Research and Science (IJAERS) https://dx.doi.org/10.22161/ijaers/3.11.30 approximately 300 data of both Kmax and ΔK along with their corresponding da/dN (calculated as per the procedure mentioned earlier). The model was applied to simulate the crack growth rate of an unknown input/output data set for load ratio of 0.5 as validation set (VS) by constructing a training set (TS) with five known input/output data sets for load ratios (R) of 0, 0.2, 0.4, 0.6 and 0.8. Start
Load training data
Set input parameters of MF for learning: 1. No. of iterations 2. error tolerance
Input training data set into ANFIS system; Start learning
Input prediction parameters & test with validation data set Predicted FCGR Start
Fig. 6: Flow chart of ANFIS hybrid learning algorithm
[Vol-3, Issue-11, Nov- 2016] ISSN: 2349-6495(P) | 2456-1908(O)
Fig. 6 shows the flow chart of ANFIS hybrid learning algorithm. Before applying ANFIS model, the preprocessing of experimental data is essential in order to achieve optimum modeling results. The input variables i.e. load ratios (R), maximum stress intensity factor (Kmax) and stress intensity factor range (ΔK) were normalized in such a way that their maximum values were normalized to unity. The crack growth rate (da/dN), which constituted the system output, was also normalized in similar manner. The numbers of membership functions (MF) were chosen to be 5-5-5 corresponding to the inputs R, Kmax and ΔK respectively. The 5 × 5 × 5 = 125 fuzzy ‘if-then’ rules constituted in which fuzzy variables were connected by T-norm (fuzzy AND) operators. The adjustment of premise and consequent parameters was made in batch mode based on the hybridlearning algorithm. The model was trained for 4000 epochs until the given tolerance was achieved. Table 2 summarizes all the characteristics of ANFIS network used during training. As per Fig. 5, layer 1 had 15 (5 × 3) nodes with 45 parameters. Layers 2, 3 and 4 had 125
(5 ) nodes each with 500 parameters associated in layer 4. 3
Table 2: Characteristics of the ANFIS network Type of membership Generalized function bell Number of input nodes (n) 3 Number of fuzzy partitions 5 of each variable (p) Total number of 15 membership functions n 125 Number of rules p
Total number of nodes Total number of parameters Number of epochs Step size for parameter adaptation
394 545 4000 0.01
The model performances during training and testing were verified by computing root mean square error (RMSE); coefficient of determination (R2) and mean percent error (MPE) defined by the following equations: p RMSE = (1 p )∑ ti − oi i =1
p 2 ∑ (ti − oi ) R 2 = 1 − i =1 p 2 ∑ (oi ) i =1
Page | 202
International Journal of Advanced Engineering Research and Science (IJAERS) https://dx.doi.org/10.22161/ijaers/3.11.30 30 MPE =
1 p t i − oi × 100 ∑ p i =1 ti
[Vol-3, Issue-11, Nov- 2016] ISSN: 2349-6495(P) 2349 | 2456-1908(O)
comparison. The crack length len vs. number of cycle (a~N) curve has been plotted in Fig. 8.
where‘t’ is the target value, ‘o’’ is the output value, and ‘p’ ‘ is the number of data items. The model was trained and tested by using MATLAB with Fuzzy Logic Toolbox. The performance of the model during training and testing was verified through three statistical indices (Eqs. 6 to 8)) and presented in Table 3. Table: 3 Performance of ANFIS model During training During testing Comp 2 2 RMSE R RMSE R -utatMPE MPE ional Time (Min. ) 0.0 0.99 0.27 0.01 0.99 0.77 384 012 85 58 29 86 96 7 V. DISCUSSION As observed from the performance table, table the MPE and RMSE values for the training data were negligible in both the cases. MPE values for testing were found to be slightly higher than those for training. The coefficient of determination was found to be close to 1.0 during training. However, its value for testing was slightly less than unity. unit Based on the above statistical performances, the trained ANFIS model was tested for load ratio of 0.5. 0.5 The predicted crack growth rates curve (for R=0.5) =0.5) obtained from ANFIS model has been compared with experimental results in Fig. Fig 7 and found to be in good agreement.
Fig. 7: Comparison of da/dN–ΔK curves for R=0.5 The numbers of cycles (fatigue life) have been calculated as per the following equation. a − ai (9) N i +1 = i +1 + Ni da dN The predicted (ANFIS) numbers of cycles are presented along with experimental results in Table 4 for quantitative www.ijaers.com
Fig.8: Comparison of predicted (ANFIS) and experimental crack length with number of cycle The performance of the model was evaluated by comparing the prediction results with the experimental findings by the following criteria: • Percentage deviation of predicted predi life from the experimental life i.e. predicted − Experiment al 0 Dev = × 100 0 Experimental •
Prediction ratio which is defined as the ratio of actual life (i.e. experimental) to predicted life i.e. Prediction ratio, Pr = actual predicted
Error bands i.e. the scatter of the predicted life in either side of the experimental life within certain error limits. Performance of the model result from first two criteria has been presented in Table 4. Table.4: Prediction results of the model Fatigue Fatigue life % Prediction life (×103 cycle) Deviation ratio (×103 Experimental ANFIS ANFIS cycle) ANFIS 76.826 78.783 –0.024 1.025 It is observed that the ANFIS model prediction is reasonable in comparison to experimental findings as far as prediction of fatigue life is concerned. concerned Further, the prediction ratio is approximately 1.0, which is adequate and also acceptable . Fig. 9 illustrates the performance of the alloy evaluated graphically under the third criteria. It is observed that the scatter of the predicted life is within ± 0.025%.
Page | 203
International Journal of Advanced Engineering Research and Science (IJAERS) https://dx.doi.org/10.22161/ijaers/3.11.30 30
Fig. 9: Error band scatter of predicted lives for R = 0.5 CONCLUSION VI. The focus of this work was to develop an ANFIS model in order to predict crack growth rate and in turn the fatigue life of 6061 Al alloy under the effect of load ratio. It has been observed that the predicted fatigue life from ANFIS model is 76.826×103 cycles whereas from experimental result it is 78.783×103 cycle. As far as performance of the model is concerned the percentage deviation of predicted fatigue life from the experimental result is –0.024 024 whereas the prediction ratio is 1.025. It can an be concluded that the adaptive neuro-fuzzy fuzzy technique (ANFIS) can be reasonably applied to predict the fatigue life under constant amplitude loading taking into account the load ratio effect. REFERENCES  P. C. Paris, and F. Erdogan, “A A critical analysis of crack Propagation law,” J. Basic Eng., Eng vol. 85, pp. 528–534, 1963.  R. G. Forman, V. E. Kearney, and R. M. Engle, “Numerical analysis of crack Propagation in cyclicloaded structures,” J. Basic Eng., vol. 89, pp. 459–464, 1967. 1967  K. Walker, “The The effect of stress ratio during crack propagation and fatigue for 2024--T3 and 7075-T6 aluminum,” ASTM STP, vol. 462, pp. 1–14, 1 1970.  D. Kujawski, “A new (ΔK+ Kmax)05 driving force parameter for crack growth in aluminum alloys,” Int. J. Fat., vol. 23, pp. 733–740, 2001.  D. Kujawski, “Enhanced Enhanced model of partial crack closure for correlation of R- ratio effects in aluminum alloys,” Int. J. Fat., vol. 23, pp. 95-102 102, 2001.  X. Huang, and T. Moan, “Improved Improved modeling of the effect of R-ratio on crack growth Rate,” Int. J. Fat., vol. 29, pp. 591-602, 2007.  S. B. Singh, and R. Kumar, “Experimental Observations of Fatigue Crack Growth in IS-1020 IS
[Vol-3, Issue-11, Nov- 2016] ISSN: 2349-6495(P) 2349 | 2456-1908(O)
Steel under nder Constant Amplitude Loading,” Int. J.Pres.Ves. Piping, vol. 53, pp. 217-227, 1993.  R. Kumar, “Investigation Investigation of Fatigue Crack Growth Under constant Amplitude Loading,” Int. J.Pres.Ves. Piping, vol. 41, pp. 179-192, 179 1990.  J. A. Lee, D.P. Almond, and B. Harris, “The use of neural networks for the prediction of fatigue lives of composite materials.” Compos. Part A: Appl. Sci. Manufact., vol. 30, pp. 1159-1169, 1999.  T. T. Pleune, and O. K. Chopra, “Using artificial neural networks to predict the fatigue life of carbon and low-alloy alloy steels,” Nucl. Eng. Des., vol. 197, pp. 1–12, 2000.  R. M. V. Pidaparti, and M. J. Palakal, “Neural Network Approach to Fatigue Crack-Growth Predictions under nder Aircraft Spectrum Loadings,” J. Aircraft, vol. 32, no. 4, pp. 825-831, 1995.  A. Fotovati, and T. Goswami, “Prediction of elevated temperature mperature fatigue crack growth rates in Ti-6Al-4V alloy – neural network approach,” Maters. Eng. Des., vol. 25, pp. 547-554, 2004.  Anon, “Standard Standard test method for measurement of fatigue crack growth rates,” ASTM E-647, In: ASTM Book of Standard, ASTM, Philadelphia, vol. 03.01, pp. 899– 926, 1996.  J. R. Mohanty, B. B. Verma, and P. K. Ray, “Prediction Prediction of fatigue crack growth and residual life using an exponential model: Part I (constant amplitude loading),” Int. J. Fat.,, vol. 31, pp. 418-424, 2009.  J. S. R. Jang, “ANFIS: ANFIS: Adaptive-network-based Adaptive fuzzy inference system,” IEEE Trans. Trans on Syst. Man Cyber., vol. 23, no. 3, pp. 665-685, 665 1993.  T. Takagi, and M. Sugeno, “Fuzzy identification of systems and its applications cations to modeling and control,” IEEE Trans. on Syst. Syst Man Cyber., vol. 15, pp. 116– 132, 1985.  M. A. Jarrah, Y. Al--Assaf, and H. El Kadi, “Neurofuzzy modeling of fatigue life prediction of unidirectional glass fiber / epoxy composite laminates,” J. Comput. Comput Mats., vol. 36, no. 6, pp. 685– 699, 2002.  S. B. Singh, and R. Kumar, “Experimental Observations of Fatigue Crack Growth in IS-1020 Steel under nder Constant Amplitude Loading,” Int. J. Pres. Ves. Piping, vol. 53, pp. 217-227, 217 1993.  P. Heuler, and W. Schuetz, “Assessment of concepts for fatigue crack initiation and propagation life prediction,” Z. Werkstofftech vol. 17, pp. 397-405, 1986. Page | 204